Impact of Volcanic Ash on Road and Airfield Surface
Daniel M Blake1,* Thomas M Wilson1 Jim W Cole1 Natalia I Deligne2 Jan M Lindsay3 1 Department of Geological Sciences, University of Canterbury, Private Bag 4800, Christchurch, New
Zealand; email@example.com, firstname.lastname@example.org, email@example.com.
2 GNS Science, 1 Fairway Drive, Avalon 5010, PO Box 30-368, Lower Hutt 5040, New Zealand; firstname.lastname@example.org.
3 School of Environment, The University of Auckland, Private Bag 92019, Auckland, New Zealand; email@example.com.
* Correspondence: firstname.lastname@example.org; Tel.: +64 21 050 1450
Abstract: Volcanic ash deposited on paved surfaces during volcanic eruptions often compromises skid resistance, which is a major component of safety. We adopt the British pendulum test method in laboratory conditions to investigate the skid resistance of road asphalt and airfield concrete surfaces covered by volcanic ash sourced from various locations in New Zealand. Controlled variations in ash characteristics include type, depth, wetness, particle size and soluble components. We use Stone Mastic Asphalt (SMA) for most road surface experiments but also test porous asphalt, line-painted road surfaces, and a roller screed concrete mix used for airfields. Due to their importance for skid resistance, SMA surface macrotexture and microtexture are analysed with semi-quantitative image analysis, microscopy and a standardised sand patch volumetric test, which enables determination of the relative effectiveness of different cleaning techniques. We find that SMA surfaces covered by thin deposits (~1 mm) of ash result in skid resistance values slightly lower than those observed on wet uncontaminated surfaces. At these depths, a higher relative soluble content for low-crystalline ash and a coarser particle size results in lower skid resistance. Skid resistance results for relatively thicker deposits (3-5 mm) of non-vesiculated basaltic ash are similar to those for thin deposits. There are similarities between road asphalt and airfield concrete, although there is little difference in skid resistance between bare airfield surfaces and airfield surfaces covered by 1 mm of ash. Based on our findings, we provide recommendations for maintaining road safety and effective cleaning techniques in volcanic ash environments.
Keywords: asphalt; concrete; runway; highway; traction; British Pendulum Tester; safety
Functional transport networks are critical for society both under normal operating conditions and in emergencies. During volcanic eruptions, transport networks may be required for the evacuation of residents, to allow sufficient access for emergency services or military personnel to
enter affected areas and for regular societal activities. Once direct threats have subsided, transport networks are crucial for both immediate and long-term recovery, including the clean-up and disposal of material, and restoration of services and commerce. It is thus imperative that effective and realistic transport management strategies are incorporated into volcanic contingency planning in areas where society and infrastructure are at risk (e.g., Auckland, New Zealand; Kagoshima, Japan; Mexico City, Mexico; Naples, Italy; Yogyakarta, Indonesia).
Volcanic eruptions produce many hazards. Damage to transport from proximal hazards such as lava flows, pyroclastic density currents and lahars is often severe, leaving ground routes impassable and facilities such as airports closed or inoperable. Volcanic ash (ejected material with particle sizes <2 mm in diameter) is widely dispersed and, although not necessarily damaging to static transport infrastructure, is generally the most disruptive of all volcanic hazards [1,2]. Even relatively small eruptions are capable of widespread disruption on ground transport and aviation, which may continue for months due to the remobilisation and secondary deposition of ash by wind, traffic or other human activities, even after an eruption has subsided.
To date studies on the impacts of volcanic hazards to society have focussed on the effects of ash [e.g. 2-13]. These studies and reports suggest four frequently occurring types of volcanic ash impacts on surface transport:
1. Reduction of skid resistance on roads and runways covered by volcanic ash 2. Coverage of road and airfield markings by ash
3. Reduction in visibility during initial ashfall and any ash re-suspension 4. Blockage of engine air intake filters which can lead to engine failure.
Despite much anecdotal evidence, detailed work to quantify the impact of ash on surface transport including roads and airfields is in its infancy [e.g. 12,14]. Quantitative, empirical evidence can inform management strategies in syn-eruptive and post-ashfall environments such as evacuation planning, safe travel advice in the recovery phase and recommended clean-up operations.
Most studies of exposed critical infrastructure have generally focussed on very large eruptions and ashfall deposits >10 mm thick, rarely reporting the effects from ashfall <10 mm thick . This presents a source of uncertainty for emergency management planning and loss assessment models, which is important, as thin deposits are more frequent and often cover larger areas . Some notable eruptions that have led to reported reduced skid resistance on roads in the past are highlighted in Table 1. It has been suggested that impacts start at ~2-3 mm ash thickness , although there have been few studies that have quantified such impacts in detail. Indeed, the limited quantitative data available from historic observations generally relates impacts to approximate depths of ash, which may not be the best metric: ash characteristics such as particle size, ash type, degree of soluble components and wetness, may influence or even control the level of skid resistance. We investigate the importance of these alternative characteristics in this paper.
road sites. Despite the widespread and frequent use of the BPT by road engineers, we are unaware of other studies that have utilised the instrument on ash-covered surfaces.
Table 1. Historical reports of reduced skid resistance following volcanic eruptions. There may be other instances described as ‘general impacts to transportation’ or which have not been recorded in the literature.
Volcano and country Year Ash thickness (mm)
Observations related to skid resistance
St Helens, United States of America 1980 17 Ash became slick when wet [17-19]
Hudson, Chile 1991 not specified Traction problems from ash on road [7,20]
Tavurvur and Vulcan, Papua New Guinea
1994 1000 Vehicles sunk and stuck in deep ash, although
passable if hardened [21-23]
Sakurajima, Japan 1995 >1 Roads slippery [22,24]
Ruapehu, New Zealand 1995-96 "thin" Slippery sludge from ash-rain mix (roads
Soufrière Hills, United Kingdom (overseas territory)
1997 not specified Rain can turn particles into a slurry of slippery mud 
Etna, Italy 2002 2-20 Traction problems, although damp and
compacted ash easier to drive on 
Reventador, Ecuador 2002 2-5 Vehicles banned due to slippery surfaces [22,27]
Chaitén, Chile 2008 not specified Reduced traction caused dam access problems
Merapi, Indonesia 2010 not specified Slippery roads caused accidents (Figure 2) and
increased journey times 
Pacaya, Guatemala 2010 20-30 Slippery roads with coarse ash 
Puyehue-Cordón Caulle, Chile 2011 >100 2WDs experienced traction problems (wet
Shinmoedake, Japan 2011 not specified Ladders very slippery 
Kelud, Indonesia 2014 1-100 Roads slippery with increased accident rate 
Sinabung, Indonesia 2014 80-100 Road travel impracticable in wet muddy ash
1.2 Skid Resistance
Skid resistance (i.e. the force developed when a tyre that is prevented from rotating slides along a pavement surface ) is a fundamental component of road safety and should be managed so that it is adequate to enable safe operation . Skid resistance is also essential for airfields to enable sufficient acceleration, deceleration and change in direction of aircraft on the surface . It has become particularly important since the advent of turbojet aircraft with their greater weight and high landing speeds [38,39]. Skid resistance is essentially a measure of the Coefficient of Friction (CoF) obtained under standardised conditions in which the many variables are controlled so that the effects of surface characteristics can be isolated .
Skid resistance of surfaces changes over time, typically increasing in the first two years following pavement construction for roads due to the wearing by traffic, and rough aggregate surfaces becoming exposed, then decreasing over the remaining pavement life as aggregates become polished .
1.2.1 Surface macrotexture and microtexture
Surface friction is primarily a result of the macrotexture and microtexture of road and airfield pavements; these are thus intrinsically linked to skid resistance. As defined by the World Road Association-PIARC in 1987 :
• Macrotexture defines the amplitude of pavement surface deviations with wavelengths from 0.5 to 50 mm.
• Microtexture is the amplitude of pavement surface deviations from the plane with wavelengths less than or equal to 0.5 mm, measured at the micron scale .
Microtexture, a property of each individual aggregate chip, contributes in particular to skid resistance for vehicles at low speed (i.e. the tyre rubber locally bonds to the surface through adhesion). Microtexture varies from harsh to polished. When a pavement is newly constructed, microtexture is particularly rough; however, once in service, microtexture changes due to the effects of traffic and weather conditions . Macrotexture, the coarse texture of pavement surface aggregates, helps to reduce the potential for aquaplaning and provides skid resistance at high speeds through the effect of hysteresis (caused by the surface projections deforming the tyre) [36,40]. Typically, if the surface binder and aggregate chips have been appropriately applied, macrotexture levels should very gradually and linearly decrease over time as the aggregate surface slowly abrades .
1.2.2 Road skid resistance
Table 2. Minimum recommended Skid Resistance Values for different road network sites, under wet conditions and measured using the British Pendulum Tester [41,44,45].
Type of site Minimum recommended
skid resistance value
Corresponding Coefficient of Friction
Difficult sites such as:
(b) Bends with radius less than 150 m on unrestricted roads
c) Gradients, 1 in 20 or steeper, of lengths >100 m
d) Approaches to traffic lights on unrestricted roads
Motorways and heavily trafficked roads in urban areas (with >2000 vehicles per day)
All other sites 45.0 0.47
Figure 1. Variation in CoF during a rain event [after 16,49-51].
Many studies have focused on snow- and rain-related crashes in northern states of the U.S. [e.g. 52-55]. We propose that parallels may be drawn between such hazards and the hazard presented by ashfall on roads. Following a review of the literature, Aström and Wallman (2001) summarise typical CoFs for different road conditions (Table 3) . The effect of hazards such as ice and snow can be substantial with most skid resistance values under such conditions falling below the minimum recommended levels (Table 2). Skid resistance is very limited under black ice conditions.
Table 3. Skid Resistance Values (SRVs) and calculated corresponding CoFs for different road conditions (adapted from ). The two measures of friction are related by the equation: CoF = (3 x SRV) / (330 – SRV) .
Type of Site Typical Skid Resistance Value Corresponding Coefficient of Friction
Dry, bare surface 69.5-82.5 0.8-1.0
Wet, bare surface 62.4-69.5 0.7-0.8
Packed snow 20.6-30.0 0.20-0.30
Loose snow / slush 20.6-47.1 (higher value when tyres
in contact with pavement) 0.20-0.50
Black ice 15.7-30.0 0.15-0.30
Loose snow on black ice 15.7-25.4 0.15-0.25
1.2.3 Airfield skid resistance
In addition to the contaminants mentioned in section 1.2.2, a common and important contaminant on airport runway surfaces is tyre rubber. With repeated aircraft landings, rubber from tyres can cover the entire surface of landing areas, filling the surface voids and reducing macrotexture and microtexture, resulting in loss of aircraft braking capacity and directional control, especially when runways are wet [38,39]. The extent of rubber tyre contaminant accumulation on runways is dependent on the volume and type of aircraft that use the airport .
Unfortunately, there is no common index for ground friction measurements on airfields. Currently, individual airport operating authorities are responsible for providing any take-off and landing performance data as a function of a braking coefficient with ground speed, and relating this data to a friction index measured by a ground device . CoF values measured by Continuous Friction Measuring Equipment (CFME) can be used as guidelines for evaluating friction deterioration of runway pavements . The CoFs for three classification levels for FAA qualified CFME operated at 65 and 95 km h-1 test speeds are shown in Table 4. There are no airfield guideline thresholds for the BPT as it only provides spot friction measurements of the surface (and is not classified as CFME). However, BPTs are sometimes used on runways and we thus summarise BPT results for airfield concrete surfaces in section 3.
Table 4. Guideline friction values for three classification levels for FAA qualified CFME operated at 65 and 95 km h-1 test speeds . Note that there are no airfield guideline thresholds for the BPT which is not CFME and only provides spot friction measurements.
65 km h-1 95 km h-1
Minim um Maintenanc e Planning New Design / Constructio n Minim um Maintenan ce Planning New Design / Constructio n
Mu Meter 0.42 0.52 0.72 0.26 0.38 0.66
Runway Friction Tester (Dynatest Consulting, Inc.)
0.50 0.60 0.82 0.41 0.54 0.72
Skiddometer (Airport Equipment Co.)
0.50 0.60 0.82 0.34 0.47 0.74
Airport Surface Friction Tester
0.50 0.60 0.82 0.34 0.47 0.74
Safegate Friction Tester (Airport Technology USA)
Griptester Friction Meter (Findlay, Irvine, Ltd.)
0.43 0.53 0.74 0.24 0.36 0.64
Tatra Friction Tester 0.48 0.57 0.76 0.42 0.52 0.67
Norsemeter RUNAR (operated at fixed 16% slip)
0.45 0.52 0.69 0.32 0.42 0.63
1.2.4 Volcanic ash and skid resistance
Due to its rapid formation, volcanic ash particles comprise various proportions of vitric (glassy, non-crystalline), crystalline or lithic (non-magmatic) particles  which are usually hard and highly angular. Volcanic ash properties are influenced by various factors, including the magma source type, distance from the vent, weather conditions and time since the eruption. Important volcanic ash properties include:
1. Particle size and surface area
2. Composition and degree of soluble components 3. Hardness and vesicularity
4. Angularity and abrasiveness 5. Wetness.
Since coarser and denser particles are deposited close to the source, fine glass and pumice shards are relatively enriched in ash fall deposits at distal locations . Newly erupted ash has coatings of soluble components [60,61] resulting from interactions with volcanic gases and their new surfaces. Mineral fragment composition is dependent on the chemistry of the magma from which it was erupted, with the most explosive eruptions dispersing high silica rhyolite rich in hard quartz fragments [62,63]. Volcanic ash is very abrasive [3,25,64-67] with the degree of abrasiveness dependent on the hardness of the material forming the particles and their shape; high angularity leads to greater abrasiveness . Most abrasion occurs from particles <500 μm in diameter, with a sharp increase in the abrasion rate from 5 to 100 μm .
Figure 2. Vehicle accident attributed to reduced skid resistance after ashfall from Merapi volcano, Indonesia, 2010 .
At airports, ash accumulation above trace amounts usually requires closure and the removal of ash from airfields before full operations can resume, both of which incur considerable expense . For example, the eruption of Mt. Redoubt volcano in Alaska in 1989 resulted in a minimum loss of US $21 million at Anchorage International airport . Many airports face closure even before ash settles on the airfield due to potential damage to aircraft by airborne ash, or solely the threat of ash in the vicinity. As such there are limited observations of ash resulting in reduced skid resistance on airfields, although it has been noted that slippery runways are one of the primary hazards to airports from volcanic eruptions .
2.1 Sample preparation
2.1.1 Volcanic ash
the Taupo Volcanic Zone. Rhyolitic ash was sourced from deposits from the Hatepe eruption in the Taupo Volcanic Zone. These three samples were pulverised (splitting and crushing was not necessary due to their smaller original sizes) and sieved to 1000 μm (Table 5). The grain size distributions for all samples are shown in Figure 3.
Table 5. Ash samples prepared for testing. Note RCL = Ruapehu Crater Lake, WICL = White Island Crater Lake.
Ash Source Ash Type Sieve Size (μm) Soluble Components Added
Lyttelton Volcanic Group
Hard Basalt 1000 No LYT-BAS1
Yes (RCL) LYT-BAS2
Yes (WICL) LYT-BAS3
106 No LYT-BAS4
Punatekahi cone, Taupo
1000 No PUN-BAS1
Yes (RCL) PUN-BAS2
Yes (WICL) PUN-BAS3
Hatepe ash, Taupo Pumiceous Rhyolite
1000 No HAT-RHY
Pupuke, Auckland Volcanic Field
1000 No PUP-BAS1
Figure 3. Mean particle size distribution analysed using a Micromeritics Saturn DigiSizer II Laser-Sizer (3x runs per sample). Note that the maximum particle sizes for the four samples that were sieved to 1000 μm are in fact <500 μm, likely due to the pulverisation process. Some particles for the LYT-BAS4 sample (sieved to 106 μm) exceed 106 μm due to the often-tabular nature of volcanic ash particles and their ability to pass through the sieve mesh when vertically orientated.
As fresh ash contains adhered soluble components, we dosed a portion of our ash samples with fluid from volcanic crater lakes to mimic the volatile adsorption processes which occur in volcanic plumes, thus enabling the effects of soluble components on skid resistance to be studied. A dosing method using fluids from the crater lakes of Ruapehu and White Island volcanoes, New Zealand, described by Broom (2010) and Wilson et al. (2012) [70,71], was used for a portion of the 1000 μm Lyttelton and Punatekahi basaltic ash samples for road testing, and Pupuke basaltic ash sample for airfield testing. The following dosing solutions were used as previous work established that they produce samples representative of real fresh volcanic ash [70,71]:
• 100% strength Ruapehu Crater Lake fluid (Table A1), i.e. no dilution, mixed at a ratio of 1:1 (ash to dosing agent)
• 20% strength White Island Crater Lake fluid (Table A1), i.e. 4 parts de-ionised water to 1 part White Island Crater Lake fluid, mixed at a ratio of 4:1 (ash to dosing agent).
We undertook a water leachate test using the method outlined by Stewart et al. (2013)  to measure the concentration of dissolved material in solution for all of the samples used and verify the effectiveness of dosing. Both 1:20 and 1:100 ratios of ash (g) to de-ionised water (ml) were used. The water leachate test findings (Figure A1) revealed that the soluble components in the samples we dosed (LYT-BAS2, LYT-BAS3, PUN-BAS2, PUN-BAS3, PUP-BAS3) were considerably higher than those that were not dosed and confirms that the samples used provide a suitable means of testing the effects of this characteristic on skid resistance. Additionally, the lowest pH values were generally recorded for the dosed samples.
2.1.2 Test surfaces
Stone Mastic Asphalt (SMA) surfaces are commonly used on modern motorways, such as in parts of the UK and on the Auckland State Highway Network in New Zealand . However, concerns have been raised about its use, as initial skid resistance may be low until the thick binder film is worn down: it sometimes takes up to two years for the material to offer an acceptable level of skid resistance [73-75]. The desire to have good macrotexture led to the development of OGPA .
2.1.3 Painted road markings
Under typical conditions, road markings reduce accident rates  as they provide continuous visual guidance of features such as road edges and centres. However, when non-mechanical markings such as paint and thermoplastics are applied, the microtexture of the road surface changes and, with thicker non-mechanical markings, the macrotexture also alters as voids in the asphalt become filled. Consequently, localised skid resistance can be substantially reduced. The skid resistance of the markings is generally lower than that for the bare pavement, although the addition of retroreflective glass beads to the surface can increase skid resistance to more acceptable levels . As little as 0.1 mm of volcanic ash may obscure road markings , meaning that drivers may unintentionally travel over marked road surfaces (e.g. such as crossing centre lines). Further accumulation may inhibit the effectiveness of rumble strips which normally cause vibrations within the vehicle.
Paint is the most common form of road marking material used in many countries, including New Zealand, and is typically applied by spraying in dry film with thicknesses varying from 70 μm to 500 μm . In New Zealand, retroreflective glass beads are often applied to longitudinal centre line paint but not to paint on the road margins . Road lines are usually re-painted once or twice a year to account for abrasion, with skid resistance decreasing as the paint fills more voids in the asphalt surface. With a typical asphalt lifespan of ~10 years, marking paint accumulation can be substantial in places . In this study we test skid resistance on SMA slabs, machine painted by Downer Group with typical road paint (Damar Bead Lock Oil Based Paint containing 63% solids), in four forms:
• 1x application (180-200 μm thick) without retroreflective glass beads
• 1x application (180-200 μm thick) with retroreflective glass beads
• 4x applications (720-800 μm thick) without retroreflective glass beads
• 4x applications (720-800 μm thick) with retroreflective glass beads.
The asphalt with one application of paint is used to replicate markings that have been heavily abraded, whereas that with four applications mimics typical marking thickness found on New Zealand roads .
2.2 Skid resistance testing
Figure 4. British Pendulum Tester (BPT) used for surface friction testing.
2.2.1 Surfaces not covered by ash
As the ASTM E303 (2013) method states, the direct values are measured as British Pendulum (Tester) Numbers (BPNs) . Typically, tests using the BPT are conducted on wet surfaces. However, as we are also investigating the effects of dry volcanic ash on skid resistance, we also ran the experiments under dry conditions. For surfaces not covered in ash, we adopted the same technique as used by the New Zealand Transport Agency (NZTA) , whereby for each test surface area, results of a minimum of five successive swings which do not differ by more than 3 BPNs are recorded. The mean of the 5 BPNs is then calculated to give a value representing skid resistance (i.e. the Skid Resistance Value (SRV)). The tests were conducted on every side of each slab to retrieve four SRVs (later averaged) for each condition. CoFs for each mean SRV are calculated using the following equation :
CoF = (3 x SRV) / (330 – SRV) (1)
2.2.2 Surfaces covered by ash
The ash characteristics analysed during experimentation and production techniques are summarised in Figure A2. For the surfaces covered in ash, we use two test methods to replicate different ash settling conditions in combination with vehicle movement effects:
type (and re-wetted if applicable) to maintain a consistent depth (and wetness). This test method mimics to some degree the effect of vehicles driving during ash fall, with ash settling on a road surface and filling any voids left by vehicle tyres before the next vehicle passes. A mean SRV is calculated by repeating the test on all four sides of each asphalt slab.
2. Eight successive swings of the pendulum are taken over each ash-covered test surface area but ash is not replenished between each swing. For each swing, the BPN is taken to be the SRV, allowing the change in skid resistance to be observed through analysis of the individual results. If the original surface has been wetted, further water is applied between each swing. To some degree, this method represents vehicle movement over an ash-covered surface in dry or wet conditions, where ashfall onto the road surface has ceased. A mean SRV is calculated for each successive swing by repeating the test on all four sides of each asphalt slab where possible.
In dry field conditions, the impact of remobilised ash might be more substantial than captured in the laboratory tests. However, some remobilisation during experimentation is achieved as a result of the pendulum arm movement and associated ash disturbance.
Following testing, the ash was cleaned from the asphalt concrete slabs by brushing and using compressed air if dry, or a combination of compressed air, water and light scrubbing if wet. Wetted slabs were then left to air-dry for 3-4 days before any further dry tests were conducted.
2.3.1 Sand patch method
This volumetric technique is standardised in the ASTM E965 (2006) method  and summarised in Figure A3. It involves a procedure for determining the average depth of pavement macrotexture by careful application of a known volume of spherical glass beads on the surface and subsequent measurement of the total area covered. The average pavement macrotexture depth is calculated using the following equation:
MTD = 4V / πD2 (2)
Where MTD = mean texture depth of pavement macrotexture (mm), V = sample volume (mm3) and D = average diameter of the area covered by the material (mm).
We use this approach to determine the macrotexture of new non-contaminated SMA surfaces and SMA surfaces that were contaminated by ash but have undergone testing (10x BPT swings) and cleaning (see section 2.2.3). The method is not suitable for the airfield concrete slabs due to there being considerably fewer voids at the macrotexture scale and thus a much larger area would be required to conduct the test.
2.3.2 Image analysis
assessed through the calculation of remaining ash coverage. The light-coloured rhyolitic volcanic ash (sample ID: HAT-RHY) was used to allow easy visual interpretation between the ash and dark-coloured asphalt concrete.
1. White paint was marked on the edge of the slabs in order to identify the same segment of the slab between each testing round.
2. A Fuji Finepix S100 (FS) digital SLR camera (with settings: Manual, ISO 800, F6.4, 10-second timer) was mounted on a tripod directly above the asphalt slab.
3. Halogen tripod worklights were used to illuminate the surface of the slab and all ambient light was blocked out using black sheeting before images were taken to keep lighting levels consistent between photos.
4. Images were analysed for percentage coverage of ash by means of ‘training’ and ‘segmentation’ using ‘Ilastik’ and ‘Photoshop’ software.
2.4 Microtexture – microscopy
A Meiji EMZ-8TRD (0.7-4.5 zoom) stereomicroscope and Lumenera Infinity 1 digital camera were used to capture images of 10 x 10 mm areas on the asphalt slabs and thus enable visual identification of remaining ash particles at a microtextural level. The microscope was mounted directly above the slab and Leica CLS 100 LED fibre-optic lighting was used to illuminate the section of interest, with all ambient light blocked using black sheeting. A portable (300 x 300 mm internal dimension) grid (with 10 mm squares) was constructed to fit securely over the slab and allow easy identification of specific segments between each testing round (Figure A4).
3. Results and Discussion
3.1 Consistent depth
Figure 6. Mean SRVs and COFs for the non-contaminated airfield concrete and airfield concrete covered in the two ash types sieved to 1000 μm. Wet and dry samples at 1, 3, 5, 7 and 9 mm thicknesses are shown. The error bars represent the standard deviation for each data set.
3.1.1 Ash type and wetness
Anecdotal observations during historical eruptions suggest that skid resistance on roads is reduced following dry unconsolidated ash accumulation. This is consistent with our results, which also reveal that reduced SRVs are particularly pronounced under dry conditions for a 1 mm thick ash layer on asphalt (Figure 5). Mean SRVs for all 1 mm thick ash types fall below the minimum recommended SRV for difficult sites (an SRV of 65). Wet 1 mm ash-covered surfaces are not necessarily more slippery than dry 1 mm ash-covered surfaces and the wet surfaces covered in 1 mm thick ash are only slightly more slippery than the wet asphalt without ash contamination.
slowed upon initial impact with the thicker deposits, producing higher than true representative SRVs. However, the comparatively low SRVs for the 5 mm thick LYT-BAS1 sample suggest that other ash characteristics are also important.
Compared to asphalt, there is less difference between SRVs for bare airfield concrete surfaces and those covered by 1 mm of ash (Figure 6), perhaps due to the initially smooth surface when bare. However, as with the asphalt, results suggest little difference in slipperiness between wet and dry surfaces with 1 mm of ash deposition. The scoriaceous and vesicular sample PUP-BAS1 exhibits especially large SRVs as thickness is increased, reinforcing our hypothesis that ash of this type is less slippery when thicker. The apparent increase in skid resistance with the addition of ash to SRV values greater than those for bare surfaces may be a function of the pendulum arm slowing upon contact.
3.1.2 Soluble components
Figure 7. Mean SRVs and CoFs for the road asphalt covered in non-dosed and dosed LYT-BAS and PUN-BAS ash sieved to 1000 μm. Both samples dosed in RCL and WICL fluid under dry and wet conditions are displayed. Due to limitations in dosing fluids and possible interference caused by the crystalline characteristics of the LYT-BAS samples, most testing was undertaken using the
PUN-BAS samples. Large quantities of freshly dosed ash samples were required for each thick ash test under wet conditions, hence only dry conditions were analysed for the 5 and 7 mm thick testing rounds. Also displayed (as red dashed lines) are the minimum recommended SRVs for different road network sites (Table 2).
Figure 8. Mean SRVs and CoFs for the airfield concrete covered in non-dosed and dosed PUP-BAS ash sieved to 1000 μm. The samples dosed in WICL fluid under both dry and wet conditions are displayed.
3.1.3 Ash particle size
improved contact between the tyre and asphalt. However, no clear correlations exist between the fine- and coarse-grained ash when at 5 mm thick, perhaps due to both types covering the asphalt surface when the tyre makes contact.
Figure 9. Mean SRVs and CoFs for the asphalt covered in coarse-grained (i.e. LYT-BAS1, 1000 μm sieved) and fine-grained (i.e. LYT-BAS4, 106 μm sieved) samples at 1 mm and 5 mm ash thickness under both dry and wet conditions. Also displayed (as red dashed lines) are the minimum recommended SRVs for different road network sites (Table 2).
3.1.4 Line-painted asphalt surfaces
Figure 10. Mean SRVs and CoFs for the road asphalt with line-painted surfaces. Conditions of no ash, 1 mm thick ash, and 5 mm thick ash (using the LYT-BAS1 ash type) were analysed under both wet and dry conditions. Also displayed (as red dashed lines) are the minimum recommended SRVs for different road network sites (Table 2).
3.1.5 Asphalt comparison
Because of increased macrotexture of the surface, higher SRVs (~ 5) were measured on the bare OGPA than the SMA slabs when wet. Similar differences in SRVs existed between the two asphalt types covered by wet volcanic ash (both at 1 mm and 5 mm depths). However, no major differences in SRVs were observed between the two asphalt types when dry, whether surfaces were covered by ash or not.
3.2 Inconsistent depth
Where ash was not replenished between each swing, SRVs represent those expected for surfaces where ashfall has ceased but where there is some traffic movement.
3.2.1 Ash types and wetness
SRV results obtained for the samples sieved to 1000 μm (at 1mm and 5 mm ash thickness) and deposited on road asphalt are shown in Figure 11. Note that tests of other thicknesses (3, 7 and 9 mm) were also conducted but these have been omitted from the figure for clarity.
Figure 11. SRVs and corresponding CoFs on asphalt covered by ash sieved to 1000 μm, under (a) dry and (b) wet conditions. Also shown are the mean SRVs for bare asphalt, taken from section 3.1. Error bars display the standard deviations for each pendulum swing number for the different sample types. Note that the first 2-3 swings over 5 mm deposits should be interpreted with caution due to possible impacts on SRVs caused by the initial contact between the pendulum slider and surface.
Despite the large standard deviations, the 5 mm thick PUN-BAS1 and HAT-RHY samples initially produced high SRVs. However, the SRVs recorded for the first 2-3 swings of the pendulum
A (Dry road)
over 5 mm thick ash should be interpreted with caution. This is due to possible interference of the thicker deposit when the pendulum slider first impacts the surface; similar circumstances may occur in the field when initial vehicles are driven into thicker ash deposits. When wet however, the SRVs are higher than the mean recorded on the bare asphalt surface, particularly for the PUN-BAS1 sample, suggesting that thicker layers of vesiculated (and especially harder) volcanic ash are perhaps initially less slippery than thin layers of ash of those ash types. Observations during our experimentation revealed that the wet 5 mm thick vesiculated deposits (PUN-BAS1 and HAT-RHY) consolidated, thus resisting major ash displacement more than for dry ash (Figure 12), even following several swings of the pendulum arm. The consolidated deposits were very firm to touch and, although further work is required to test this, it is suggested that light vehicles would be able to drive over the surface without sinking substantially.
Figure 12. Dry ash displacement from the BPT slider-surface interface after 8x swings of the pendulum arm for (a) SMA, and (b) airfield concrete. Dry ash was displaced from the surface more readily than wet ash. Note that white lines indicate length of slider contact path (i.e. 125 mm).
Very similar patterns in skid resistance were observed for the airfield concrete surfaces where ash was not replenished between swings. The main difference was that the initially high SRVs for the scoriaceous sample (PUP-BAS) decreased more quickly with pendulum swings, most likely due to the ash being more easily displaced from the smoother concrete surface than for asphalt.
3.2.2 Ash particle size
No major changes were observed for the fine-grained basaltic ash samples (LYT-BAS4) over the course of the eight pendulum swings on asphalt, other than a gradual increase in SRVs over time, particularly for the dry ash at 1 mm thickness as observed for the coarse-grained samples (Figure 11a). As with the testing where ash was replenished, here SRVs for the fine-grained ash samples were generally slightly higher than those for coarse-grained samples, suggesting that fine-grained ash is a little less slippery than coarser material.
3.2.3 Soluble components
The testing involving non-replenished dosed ash confirmed the key finding already discussed during replenished testing (section 3.1.2); non-crystalline ash containing a higher soluble component content generally produces lower SRVs than undosed ash. However, with an increasing number of swings of the pendulum, this trend becomes less pronounced, particularly under wet conditions where the effect of adding water between each test leaches the samples, thus reducing the soluble component content of the ash.
3.2.4 Line-painted asphalt surfaces
Line-painted asphalt surfaces covered in ash (Figure 13) produce relatively low SRVs. Although the first 2-3 swings involving 5 mm thick ash are not considered, it is evident that wet painted surfaces are generally slightly more slippery than painted dry surfaces. The trend of quick SRV recovery (as seen in section 3.2.1) is also evident under dry line-painted conditions, when compared to wet conditions which remain slippery for longer. Under dry conditions, the addition of retroreflective glass in the line-paint appears to aid the recovery of skid resistance over time (as shown by the rising green and orange lines for the latter swings in Figure 13a). However, this trend is not evident for wet conditions.
B (Wet A (Dry
Figure 13. SRVs and corresponding CoFs for line-painted asphalt surfaces covered in 1 mm or 5 mm thick LYT-BAS1, under (a) dry, and (b) wet conditions. Only one test was conducted on each surface type due to the availability of line-painted slabs. Therefore, no standard deviations were calculated and the results should be treated with some caution. Note that the initial 2-3 swings over the 5 mm deposits should be treated with particular caution.
3.3 Surface Macro and Microtexture
3.3.1 Ash displacement and removal
The results for mean macrotexture depth calculated using the sand patch method for the bare, clean, new asphalt surface and the asphalt surface following dry testing and brushing, and cleaning with compressed air after contamination are shown in Table 6.
Table 6. Mean macrotexture depth of asphalt slab before and after testing/cleaning, calculated using the ASTM sand patch method, and percentage ash surface coverage.
Asphalt Concrete Slab Condition Mean Macrotexture Depth (mm)
Ash surface coverage (%)
Bare, clean and new 1.37 0
Ashed, 10x BPT swings - 81
Ashed, 10x BPT swings and
brushed (10x strokes) 0.99 40
Cleaned with compressed air 1.29 <1
Figure 14. Macrotexture image sequence for asphalt. (a) Clean new slab, (b) covered with 1 mm rhyolitic ash (100% surface coverage), (c) after 10x BPT swings (81% surface ash coverage), (d) after cleaning with 10x brush strokes (40% surface ash coverage), (e) after cleaning with compressed air (<1% surface ash coverage). The macrotexture of the surface is visibly affected in images b-d with much ash remaining between the asphalt’s aggregate pore spaces, even after 10x BPT swings and cleaning using a brush.
Cleaning using high-pressure water spraying and brushing was more effective than brushing alone at removing ash (<1% surface ash coverage afterwards). However, this approach requires large quantities of water and the microscope imagery revealed that some small particles of ash remain on the surface, which would perhaps still reduce skid resistance somewhat. Field observations from Kagoshima, Japan, where high quantities of only low-pressure water are used to clean road surfaces indicates that some ash remains on the road surfaces even immediately after
cleaning . Furthermore, clearing ash from roads using water may cause some drainage systems to become blocked , potentially resulting in surface water flooding.
3.3.2 Temporal change of skid resistance on bare asphalt surfaces
In normal conditions, the skid resistance of bare asphalt surfaces changes over time. Typically, during the first two years following construction it increases as the surface is worn by traffic and rough aggregate surfaces become exposed, and then decreases over time as the aggregates become more polished . The initial trend of increasing skid resistance was confirmed during our testing of the bare wet asphalt and concrete slabs before and after contamination with ash (but following cleaning), particularly so for the asphalt (Figure 5). We suggest that the abrasive properties of volcanic ash accelerates these processes, especially for our testing as all ash particles were <500 μm in diameter (see section 1.2.4). Following testing, the SRV of bare wet asphalt had increased by around 5. The microscopy imagery showed that the lustrous film on the new asphalt slabs had been removed during BPT experimentation (Figure 15).
Figure 15. Microscope images on the same segment of asphalt, (a) on the new slab and (b) after contamination with volcanic ash and cleaning with compressed air. Much of the shiny film visible on the surface of the new asphalt has been removed. Note that the length of the white lines is 10 mm and that lighting conditions and microscope settings were consistent for both images.
4.1 Key findings
Our experiments suggest that the following lead to particularly reduced skid resistance on asphalt road surfaces and may thus lead to slippery surfaces following volcanic ashfall:
• Thin (~1 mm deep) layers of relatively coarse-grained ash, with ash type having little effect at this depth (average SRVs of 55-65).
• Thicker (~ 5 mm deep) layers of hard, non-vesiculated ash (average SRVs of 55-60).
• Ash of low crystallinity or containing a high degree of soluble components (average SRVs ~5 lower than for ash that has undergone substantial leaching).
• Line-painted surfaces that are either dry or wet but covered by thin layers of ash, particularly when paint does not incorporate retroreflective glass beads (average SRVs of ~55).
Importantly, the largest change in skid resistance for surfaces that became covered by ash occurs during dry conditions, where SRVs fall to levels just below those for wet non-contaminated surfaces, with similar SRVs as the wet contaminated surfaces. This large reduction in skid resistance
may not be expected by motorists who may consequently not adjust driving, potentially resulting in high accident rates. As time goes on, wet ash deposits on roads are most likely to lead to reduced skid resistance, particularly for thicker deposits as these remain slippery for longer (typical SRVs of around 55).
Similarities exist for airfield surfaces and the second and third bullet points above are especially true for the concrete surface type. The following additional key findings are also drawn:
• There is little difference in skid resistance between bare airfield surfaces and those covered by ~1 mm of ash.
• Low crystalline ash containing high soluble components may result in SRVs of up to 20 less than non-dosed samples, particularly if the ash is thicker (~7-9 mm depth).
• Ash is more readily displaced on smoother airfield concrete than road asphalt causing SRVs to recover to ‘typical non-contaminated’ values at a faster rate with consistent traffic flow.
4.2 Recommendations for road safety
Based on skid resistance analysis, we make the following recommendations to increase road safety in areas with volcanic ashfall exposure of ≤ 5 mm depth:
• During initial ash fall, vehicle speed (or advisory speed) should immediately be reduced to levels below those advised for driving in very wet conditions on that road, whether the surface is wet or dry. Wet ash is not necessarily more slippery than dry ash, at least initially.
• Fresh ash contains more soluble components, which results in lower skid resistance values than for leached ash. Therefore, it is important to advise motorists promptly of any restrictions.
• Particular caution should be taken on dry surfaces that become covered by coarse-grained ash as skid resistance will reduce substantially from what occurs on dry non-contaminated surfaces. The slipperiness of dry surfaces with such contamination may not be expected by motorists (skid resistance values will be similar as for wet fresh ash and slightly less than for wet non-contaminated conditions).
• Road markings may be hidden from view, impacting road safety through lack of visual and audio guidance of road features. Areas of road that are line-painted and covered in thin ash are especially slippery. Motorcyclists and cyclists in particular should take extreme care.
4.3 Airport safety
We do not make any specific recommendations for airport safety related to concrete airfield surfaces, although it is highlighted that extensive efforts may be required to clean airfield surfaces as has occurred following historical eruptions (e.g. Chaitén 2008 , Kelud 2014 ). It is likely that airports will remain closed until all ash has been cleared from runways due to other potential impacts such as damage to aircraft turbine engines. Our results suggest that residual ash of minimal depths on concrete airfield surfaces is likely to have little effect on skid resistance. However, airport managers should be aware that freshly erupted ash or ash that has not been leached (i.e. containing higher soluble components) will likely be more slippery than that which has persisted in the environment for some time. As with road asphalt, wet ash is not necessarily more slippery than dry ash on airfield concrete and any restrictions implemented should thus be in place for both conditions.
4.4 Recommendations for cleaning
The following advice for road cleaning is given based on our studies of macrotexture and microtexture and from the observations during small-scale cleaning conducted on our slabs between skid resistance tests:
• Brushing alone will not restore surfaces to their original condition in terms of skid resistance. Following simple brushing practices on asphalt roads, the macrotexture depth may be around one third less than the original depth and ~40% ash coverage may occur on the surface.
• If surfaces are dry and contaminated with dry ash, air blasting combined with suction and capture of loosened ash, is an effective way to remove ash from macrotextural pores. Minor quantities of ash may remain at the microtextural level although this is deemed too low to substantially affect skid resistance.
• If surfaces are wet, a combination of water spraying and brushing and/or air blasting (with suction and ash capture) is an effective way to remove most ash and restore surface skid resistance. However, large quantities of water are required and some ash will remain in the asphalt pore spaces, especially if low-pressure water is used. Care should be taken if using water for ash removal due to the potential for blockage of some drainage systems.
Ash remobilisation should be carefully considered prior to cleaning. Extensive (and often expensive) cleaning efforts may be useless if ash continues to fall or is remobilised from elsewhere and deposited onto roads and airfields.
thanks also go to the people who provided support with the laboratory set-up at various stages, including technician support from Rob Spiers, Matt Cockcroft, Chris Grimshaw and Sacha Baldwin-Cunningham. We also thank researchers Emily Lambie, Rinze Schuurmans, Alec Wild and Alistair Davies for their assistance with sample preparation and skid resistance testing.
Author Contributions: All authors contributed to the manuscript. DB conducted the majority of the planning, research and laboratory testing, and also led the writing and editing of the article. TW assisted DB in the development of the methodology including potential experimental approaches. TW, JC, ND and JL conducted multiple reviews of the article prior to submission.
Conflicts of Interest: The authors declare no conflicts of interest.
Table A1. Concentration of elements in the Ruapehu and White Island Crater Lake fluids at the strength used to dose the ash (after Broom 2010, Wilson 2012).
Ruapehu Crater Lake (100% strength)
White Island Crater Lake (20% strength)
Aluminium (Al) 370 965
Boron (B) 17.2 28.6
Bromine (Br) 10.8 44.2
Calcium (Ca) 909 823
Chlorine (Cl) 5,568 19,452
Fluorine (F) 133 1,518
Iron (Fe) 424 179
Potassium (K) 90 686
Lithium (Li) 0.77 5.60
Magnesium (Mg) 1,067 1,325
Sodium (Na) 660 3,372
Ammonia (NH3) 13.0 24.8
Sulphate (SO42-) 7,988 4,952
Figure A1. Water leachate results showing relative soluble components (expressed as Electrical Conductivity (EC) and Total Dissolved Solids (TDS)), and pH. (a) 1:100 ash to de-ionised water, (b) 1:20 ash to de-ionised water.
1. Johnston, D.M.; Daly, M. Auckland erupts!! New Zealand Science Monthly 1995, 8:10, pp.6-7.
2. Wilson, G.; Wilson, T.M.; Deligne, N.I.; Cole, J.W. Volcanic hazard impacts to critical infrastructure: a review. J Volcanol Geotherm Res 2014, 286, pp.148-182.
3. Blong, R.J. Volcanic hazards: a sourcebook on the effects of eruptions. Academic Press Inc: New South Wales, Australia 1984.
4. Guffanti, M.; Mayberry, G.C.; Casadevall, T.J.; Wunderman, R. Volcanic hazards to airports. Nat Hazards 2009, 51, pp.287-302.
5. Wilson, T.; Daly, M.; Johnston, D. Review of impacts of volcanic ash on electricity distribution systems, broadcasting and communication networks. Auckland Engineering Lifelines Group, Auckland Regional Council Technical Publication No. 051, 2009.
6. Horwell, C.J.; Baxter, P.J.; Hillman, S.E.; Damby, D.E.; Delmelle, P.; Donaldson, K.; Dunster, C.; Calkins, J.A.; Fubini, B.; Hoskuldsson, A.; Kelly, F.J.; Larsen, G.; Le Blond, J.S.; Livi, K.J.T.; Mendis, B.; Murphy, F.; Sweeney, S.; Tetley, T.D.; Thordarson, T.; Tomatis, M. Respiratory health hazard assessment of ash from the 2010 eruption of Eyjafjallajökull volcano, Iceland: a summary of initial findings from a multi-centre laboratory study. IVHHN and Durham University, Durham, UK, 2009.
7. Wilson, T.M.; Stewart, C.; Cole, J.W.; Dewar, D.J.; Johnston, D.M.; Cronin, S.J. The 1991 eruption of Volcan Hudson, Chile: impacts on agriculture and rural communities and long-term recovery. GNS Science Report 2009/66, 99p, 2011.
8. Dunn, M.G. Operation of gas turbine engines in an environment contaminated with volcanic ash. J Turbomachinery 2012, 134:5, 18p.
9. Wardman, J.; Sword-Daniels, V.; Stewart, C.; Wilson, T. Impact assessment of the May 2010 eruption of Pacaya volcano, Guatemala. GNS Science Report 2012/09, 2012.
10. Wilson, T.M.; Stewart, C.; Sword-Daniels, V.; Leonard, G.S.; Johnston, D.M.; Cole, J.W.; Wardman, J.; Wilson, G.; Barnard, S.T. Volcanic ash impacts to critical infrastructure. Phys Chem Earth 2012, 45-46, pp.5-23.
11. Stewart, C.; Horwell, C.; Plumlee, G.; Cronin, S.; Delmelle, P.; Baxter, P.; Calkins, J.; Damby, D.; Mormon, S.; Oppenheimer, C. Protocol for analysis of volcanic ash samples for assessment of hazards from leachable elements. IAVCEI, IVHHN, Cities on Volcanoes Commission, USGS, GNS Science, 2013.
12. Blake, D.M.; Wilson, T.M.; Gomez, C. Road marking coverage by volcanic ash. Environ Earth Sci 2016, 75:1348, pp.1-12.
13. Hayes, J.; Wilson, T. M.; Deligne, N. I.; Cole, J.; Hughes, M. A model to assess tephra clean-up requirements in urban environments. J Appl Volc 2017, 6:1.
14. Blake, D.M.; Wilson, T.M.; Stewart, C. Visibility in airborne volcanic ash: considerations for surface transportation using a laboratory-based method. Nat Hazards in review.
15. Pyle, D.M. The thickness, volume and grainsize of tephra fall deposits. Bull Volc 1989, 51, pp.1-15. 16. Wilson, D.J. An analysis of the seasonal and short-term variation of road pavement skid resistance. PhD
Thesis, Department of Civil and Environmental Engineering, University of Auckland, Auckland, New Zealand, 2006.
17. Warrick, R.A. Four communities under ash. Institute of Behavioural Science, University of Colorado, Boulder, U.S., 1981.
University of Canterbury.
19. Cole, J.W.; Sabel, C.E.; Blumenthal, E.; Finnis, K.; Dantas, A.; Barnard, B.; Johnston, D.M. GIS-based emergency and evacuation planning for volcanic hazards in New Zealand. Bull NZ Soc Earthquake Engineering 2005. 38:2, pp.149-164.
20. Wilson, T.M. Unpublished field notes from the Hudson eruption field visit. University of Canterbury, Christchurch, New Zealand, 2009.
21. Nairn, I.A. The effects of volcanic ash fall (tephra) on road and airport surfaces. GNS Science Report 2002/13, 32p, 2002.
22. Barnard, S. The vulnerability of New Zealand lifelines infrastructure to ashfall. PhD Thesis, Hazard and Disaster Management, University of Canterbury, Christchurch, New Zealand, 2009.
23. Stammers, S.A.A. The effects of major eruptions of Mt Pinatubo, Philippines and Rabaul Caldera, Papua New Guinea, and the subsequent social disruption and urban recovery: lessons for the future. MSc Thesis, Geology, University of Canterbury, New Zealand, 2000.
24. Durand, M.; Gordon, K.; Johnston, D.; Lorden, R.; Poirot, T.; Scott, J.; Shephard, B. Impacts and responses to ashfall in Kagoshima from Sakurajima Volcano – lessons for New Zealand. GNS Science Report 2001/30, 53p, 2001.
25. Johnston, D.M. Physical and social impacts of past and future volcanic eruptions in New Zealand. PhD Thesis, Earth Science, Massey University, Palmerston North, New Zealand, 1997.
26. Small explosion produces light ash fall at Soufriere Hills volcano, Montserrat. United States Geological Survey. Available online: https://volcanoes.usgs.gov/ash/ashfall.html#eyewitness (accessed on 20 October 2015).
27. Leonard, G.S.; Johnston, D.M.; Williams, S.; Cole, J.W.; Finnis, K.; Barnard, S. Impacts and management of recent volcanic eruptions in Ecuador: lessons for New Zealand. GNS Science Report 2005/20, 2006.
28. Wilson, T.M.; Cole, J.; Johnston, D.; Cronin, S.; Stewart, C.; Dantas, A. Short- and long-term evacuation of people and livestock during a volcanic crisis: lessons from the 1991 eruption of Volcán Hudson, Chile. J Appl Volc 2012, 1:1, pp.1-11.
29. Wilson, T.M. Unpublished field notes from the Chaitén eruption field visit. University of Canterbury, Christchurch, New Zealand, 2008.
30. BORDA respond to Merapi disaster. Bremen Overseas Research and Development Association, South East Asia, Jamaludin, D., 2010. Available online:
http://www.borda-sea.org/news/borda-sea-news/article/borda-respond-to-merapi-disaster.html (accessed on 20 October 2015).
31. Wilson, T.; Outes, V.; Stewart, C.; Villarosa, G.; Bickerton, H.; Rovere, E.; Baxter, P. Impacts of the June 2011 Puyehue-Cordón Caulle volcanic complex eruption on urban infrastructure, agriculture and public health. GNS Science Report 2012/20, 88p, 2013.
32. Wilson, T.M. Unpublished field notes from the Shinmoedake eruption field visit. University of Canterbury, Christchurch, New Zealand, 2011.
33. Blake, D.M.; Wilson, G.; Stewart, C.; Craig, H.M.; Hayes, J.L.; Jenkins, S.F.; Wilson, T.M.; Horwell, C.J.; Andreastuti, S.; Daniswara, R.; Ferdiwijaya, D.; Leonard, G.S.; Hendrasto, M.; Cronin, S. The 2014 eruption of Kelud volcano, Indonesia: impacts on infrastructure, utilities, agriculture and health. GNS Science Report 2015/15, 139p, 2015.
35. Highway Research Board. National Cooperative Highway Research Program Synthesis of Highway Practice 14: skid resistance. National Academy of Sciences, Washington D.C., 1972.
36. Dookeeram, V.; Nataadmadja, A.D.; Wilson, D.J.; Black, P.M. The skid resistance performance of different New Zealand aggregate types. IPENZ Transportation Group Conference, Shed 6, Wellington, New Zealand, 23-26 March 2014.
37. Industry best practices manual for timely and accurate reporting of runway surface conditions by ATS/AIS to flight crew. International Civil Aviation Organisation, Regional Aviation Safety Group (Asian and Pacific Region), 2013. Available online:
http://www.icao.int/APAC/Documents/edocs/FS-07IBP%20Manual%20on%20Reporting%20of%20Runwa y%20Surface%20Condition.pdf (accessed on 02 October 2015).
38. Measurement, construction and maintenance of skid-resistant airport pavement surfaces. Advisory Circular 150/5320-12C, U.S. Department of Transportation, Federal Aviation Administration, 1997. Available online:
http://www.faa.gov/documentLibrary/media/advisory_circular/150-5320-12C/150_5320_12c.PDF (accessed on 03 October 2015).
39. Airport runways: skid resistance and rubber removal. Blastrac, The Netherlands, 2015. Available online: www.theairportshow.com/Portal/assets/.../BrochureAirport_LR.pdf.aspx (accessed 05 October 2015). 40. Wilson, D.J.; Chan, W. The effects of road roughness (and test speed) on GripTester measurements. New Zealand
Transport Agency Research Report 523, Clearway Consulting Ltd., Auckland, New Zealand, 2013. 41. Asi, I. Evaluating skid resistance of different asphalt concrete mixes. Build Environ 2007, 42:1, pp.325-329. 42. World Road Association-PIARC. Technical committee report on road surface characteristics, Permanent
International Association of Road Congress. Proceedings of the 18th World Congress, Brussels, Belgium, 1987.
43. Ergun, M.; Iyinam, S.; Iyinam, F. Prediction of road surface friction coefficient using only macro- and microtexture measurements. J Transp Engineering 2005, 131, pp.311-319.
44. British Pendulum Manual: Operation manual of the British Pendulum Skid Resistance Tester. Wessex
Engineering Ltd., United Kingdom, 2000.
45. Skid tester: AG190. Impact Test Equipment Ltd., Impact, 2010. Available online: http://www.impact-test.co.uk/docs/AG190_HB.pdf (accessed on 04 November 2014).
46. Benedetto, J. A decision support system for the safety of airport runways: the case of heavy rainstorms. Transp Res Part A: Policy and Practice 2002, 8, pp.665-682.
47. Andrey, J. Relationships between weather and traffic safety: past, present and future directions. Climatological Bull 1990, 24, pp.124-136.
48. Cova, T.; Conger, S. Transportation hazards. In Transportation Engineers’ Handbook, Kutz, M. Eds.; Centre for Natural and Technological Hazards, University of Utah, 2003.
49. Bennis, T.A.; De Wit, L.B. PIARC State-of-the-art on Friction and IFI. Paper presented at the 1st Annual Australian Runway and Roads Friction Testing Workshop, Sydney, Australia, 2003.
50. Persson, B.N.J.; Tartaglino, U.; Albohr, O. Rubber friction on wet and dry road surfaces: the sealing effect. Phys Rev B 2005, 71.
52. Qin, X.; Noyce, D.; Lee, C.; Kinar, J.R. Snowstorm event-based crash analysis. Transp Res Rec 2006, 1948, pp.135-141.
53. Khattak, A.J.; Knapp, K.K. Interstate highway crash injuries during winter snow and non-snow events. Transp Res Board 2001, 1746, pp.30-36.
54. Oh, S.; Chung, K.; Ragland, D.R.; Chan, C. Analysis of wet weather related collision concentration locations: empirical assessment of continuous risk profile. In Proceedings of the 88th Annual Meeting of the Transportation Research Board, Transportation Research Board, Washington D.C, U.S., 2009.
55. Abdel-Aty, M.; Ekram, A-A.; Huang, H.; Choi, K. A study on crashes related to visibility obstruction due to fog and smoke. Accident Analysis and Prevention 2011, 43:5, pp.1730-1737.
56. Aström, H.; Wallman, C. Friction measurement methods and the correlation between road friction and traffic safety: a literature review. Swedish National Road and Transport Research Institute (VTI), Linköping, Sweden, 2001.
57. Lester, T. Pedestrian slip resistance testing: AS/NZS 3661.1:1993. Opus International Consultants Ltd. Lower Hut, Wellington, New Zealand, 2014.
58. RuFAB – Runway friction characteristics measurement and aircraft braking: volume 3, functional friction.
European Aviation Safety Agency, Research Project EASA 2008/4, BMT Fleet Technology Limited, Kanata, Ontario, Canada, 2010. Available online:
https://easa.europa.eu/system/files/dfu/Report%20Volume%203%20-%20Functional%20friction.pdf (accessed on 05 October 2015).
59. Sarna-Wojcicki, A.M.; Shipley, S.; Waitt, R.B.; Dzurisin, D.; Wood, S.H. Areal distribution, thickness, mass, volume, and grain size of air-fall ash from the six major eruptions of 1980. In The 1980 Eruptions of Mount Saint Helens, Lipman P.W.; Mullineaux, D.R. Eds.; USGS Numbered Series 1250, Washington, pp.577-600, 1981.
60. Matsumoto, H.; Okabyashi, T.; Mochihara, M. Influence of eruptions from Mt. Sakurajima on the deterioration of materials. In Proceedings Kagoshima International Conference on Volcanoes, pp.732-735, 1988. 61. Delmelle, P.; Villiéras, F.; Pelletier, M. Surface area, porosity and water adsorption properties of fine
volcanic ash particles. Bull Volc 2005, 67, pp.160-169.
62. Heiken, G.; Wohletz, K. Volcanic ash. University of California Press, Berkeley, 1985.
63. Wardman, J.B.; Wilson, T.M.; Bodger, P.S.; Cole, J.W.; Johnston, D.M. Investigating the electrical conductivity of volcanic ash and its effect on HV power systems. Phys Chem Earth 2012, 45-46, pp.128-145.
64. Labadie, J.R. Volcanic ash effects and mitigation. Adapted from a report prepared in 1983 for the Air Force Office of Scientific Research and the Defence Advanced Research Projects Agency, 1994.
65. Heiken, G.; Murphy, M.; Hackett, W.; Scott, W. Volcanic hazards to energy infrastructure-ash fallout hazards and their mitigation. World Geothermal Congress, Florence, Italy, pp.2795-2798, 1995. 66. Miller, T.P.; Casadevall, T.J. Volcanic ash hazards to aviation. In Encyclopedia of Volcanoes, 1st ed.;
Sigurdsson, H.; Houghton, B.; Rymer, H.; Stix, J.; McNutt, S., Eds.; Academic Press, San Diego, CA, United States, pp.915-930, 1999.
67. Gordon, K.D.; Cole, J.W.; Rosenberg, M.D.; Johnston, D.M. Effects of volcanic ash on computers and electronic equipment. Nat Hazards 2005, 34, pp.231-262.
69. Tuck, B.H.; Huskey, L.; Talbot, L. The economic consequences of the 1989-90 Mt. Redoubt eruptions. Institute of Social and Economic Research, University of Alaska, Anchorage, 1992.
70. Broom, S.J. Characterisation of “pseudo-ash” for quantitative testing of critical infrastructure components with a focus on roofing fragility. BSc Thesis, University of Canterbury, Christchurch, New Zealand, 2010. 71. Wilson, G.; Wilson, T.; Cole, J.; Oze, C. Vulnerability of laptop computers to volcanic ash and gas. Nat
Hazards 2012, 63, pp.711-736.
72. Boyle, T. Skid resistance management on the Auckland State Highway Network. Transit New Zealand, 2005. Available online:
http://www.nzta.govt.nz/resources/surface-friction-conference-2005/8/docs/skid-resistance-management-auckland-state-highway-network.pdf (accessed on 15 June 2015).
73. Bastow, R.; Webb, M.; Roy, M.; Mitchell, J. An investigation of the skid resistance of stone mastic asphalt laid on a rural English county road network. Transit New Zealand, pp.1-16, 2004. Available online:
http://www.nzta.govt.nz/resources/surface-friction-conference-2005/7/docs/investigation-skid-resistance-stone-mastic-asphalt-laid-rural-english-county-road-network.pdf (accessed 16 June 2015).
74. ‘Hidden menace’ on UK’s roads. BBC News, 2015. Available online:
http://news.bbc.co.uk/2/hi/programmes/file_on_4/4278419.stm (accessed 12 February 2015). 75. Get a grip: Motorcycle road safety. Daily Telegraph, 2008. Available online:
http://www.telegraph.co.uk/motoring/motorbikes/2750422/Motorcycle-road-safety-Get-a-grip.html (accessed 12 February 2015).
76. NZRF. Road marking IS road safety, Potters Asia Pacific. New Zealand Road Marking Federation Inc. Conference, 2005.
77. NZRF. NZRF Roadmarking materials guide. New Zealand Roadmarkers Federation Inc. Auckland, New Zealand, 2009.
78. Downer Group, Christchurch, New Zealand. Personal communication (by email) with roading supervisor, December 2014 – January 2015.
79. ASTM E303. Standard test method for measuring surface frictional properties using the British Pendulum Tester. ASTM E303-93 (Reapproved 2013), 2013.
80. TNZ. Standard test procedure for measurement of skid resistance using the British Pendulum Tester, Report TNZ T/2:2003. Transit New Zealand, New Zealand, 2003.
81. Hill, D.J. Filtering out the ash: mitigating volcanic ash ingestion for generator sets. MSc Thesis, Hazard and Disaster Management, University of Canterbury, Christchurch, New Zealand, 2014.
82. ASTM E965. Standard test method for measuring pavement macrotexture depth using a volumetric technique. ASTM E965-96 (Reapproved 2006), 2006.